PRL 114, 166404 (2015)
week ending 24 APRIL 2015
Topological Properties and the Dynamical Crossover from Mixed-Valence to Kondo-Lattice Behavior in the Golden Phase of SmS Chang-Jong Kang,1' Hong Chul Choi,1 Kyoo Kim,1'2 and B. I. Min1 ’ 1Department o f Physics, Pohang University o f Science and Technology, Pohang 790-784, Korea cjCCMR, Pohang University o f Science and Technology, Pohang 790-784, Korea (Received 9 December 2014; published 22 April 2015) We have investigated temperature-dependent behaviors of electronic structure and resistivity in a mixedvalent golden phase of SmS, based on the dynamical mean-field-theory band-structure calculations. Upon cooling, the coherent Sm 4 / bands are formed to produce the hybridization-induced pseudogap near the Fermi level, and accordingly the topology of the Fermi surface is changed to exhibit a Lifshitz-like transition. The surface states emerging in the bulk gap region are found to be not topologically protected states but just typical Rashba spin-polarized states, indicating that SmS is not a topological Kondo semimetal. From the analysis of anomalous resistivity behavior in SmS, we have identified universal energy scales, which characterize the Kondo-mixed-valent semimetallic systems. DOI: 10.1103/PhysRevLett. 114.166404
PACS numbers: 71.27.+a, 71.18.+y, 75.30.Mb
Kondo and mixed-valent physics in strongly correlated 4/-electron systems have been the subject of longstanding controversy. The subjects include various interesting phe nomena such as p-wave superconductivity and non-Fermiliquid behavior in heavy-fermion systems [1-3], and recently proposed topological Kondo insulator behavior in a typical mixed-valent insulator SmB6 [4-14], The topo logical Kondo insulator of our present interest has attracted a great deal of recent attention. However, the realization of the topological properties in SmB6 is still under debate. One immediate question is whether or not a similar mixedvalent system, SmS, also has the topological properties. Indeed, the mixed-valent golden phase of SmS (p-SmS) was reported to be a topological Kondo semimetal , SmS has been studied for the last four decades [16-37], but there remain several issues still unresolved. SmS crystallizes in a face-centered-cubic (fee) structure of rock-salt (NaCl) type. At the ambient pressure, SmS has a so-called black phase, which is a semiconductor with indirect and direct band gaps of 90 meV and 0.4 eV, respectively , In the black phase of SmS (b-SmS), the valence state of Sm is divalent (2+), and so the system is nonmagnetic. Under high pressure above 6.5 kbar, SmS undergoes a first-order isostructural phase transition from fr-SmS to p-SmS, in which Sm ions are mixed valent with the average valency of 2.6 H— 2.8+ [25,26]. This isostruc tural transition is accompanied by the volume collapse by as much as 15% , as shown in Fig. 1(b). The energy gap decreases monotonically with increasing pressure. It is controversial whether p-SmS has a real gap or a pseudogap [27,28], The resistivity behavior of p-SmS is quite anomalous in the sense that the overall behavior is Kondo-lattice-like but it exhibits a couple of abnormal hump structures [33-37]. Applying pressure further, p-SmS has a magnetic instability at about 19.5 kbar with the 0031-9007/15/114(16)/166404(5)
antiferromagnetic order [31-33], Above 19.5 kbar, the resistivity shows a metallic behavior and the valence state of Sm increases toward 3+ , There have been several reports on the density-functionaltheory (DFT)-based band-structure study of SmS [15-17]. But even the ground-state insulating nature of b-SmS is not properly described by the DFT-based schemes, and so advanced methods like the dynamical mean-field theory (DMFT) should be employed to investigate the topological properties in p-SmS, which has strongly correlated 4 / electrons. Here, we have investigated electronic structures of SmS, based on the DMFT scheme. First, we have shown that the electronic properties of /?-SmS are described properly only by the DMFT scheme. Then, we have examined the T-dependent electronic structure evolution in p-SmS. Upon cooling, the 4 / states form the coherent 4 / bands with a pseudogap feature near the Fermi level (E F), and accordingly the topology of the Fermi surface (FS) is changed, which is reflected well in the anomalous resistivity
FIG. 1 (color online). Isostructural phase transition in SmS. (a) Bulk and surface Brillouin zones (BZs) of fee SmS. (b) The pressure dependence of the lattice constant and the Sm valence state of SmS (data taken from Ref. ).
© 2015 American Physical Society
PRL 114, 166404 (2015)
week ending 24 APRIL 2015
FIG. 2 (color online). Electronic structure of g-SmS (a = 5.6 A), (a) The DMFT band structure at T = 13 K. (b) Surface band structure obtained by the model slab calculation based on the DFT band structure. The surface states in the inset manifest a typical Rashba splitting with a tiny gap, and so they are not topologically protected states, (c) T-dependent band structures in the DMFT scheme. Upon cooling, the coherent Sm 4 / band emerges near EF, and the hybridization gap appears below T = 26 K. (d) T-dependent FS evolution in the DMFT scheme, which is compared with the DFT FS with 10 times enhanced SOC scheme of the Sm 4 / electron (top left) . Upon cooling, Y-centered 4-band pockets are reduced, while /-band pockets emerge at V.
behavior in g-SmS. We have demonstrated that the surface states realized in